Ultrason in the web: www.ultrason.de
Ultrason E, S, P
The Ultrason resins are amorphous thermoplastics
derived from polyethersulfone ( PESU), polysulfone
( PSU) and polyphenylsulfone ( PPSU) and offer very
high resistance to heat. Their wide spectrum of ben-
eficial properties allows them to be molded into high-
quality engineering parts and high-load mass-produced
articles. They can be processed by almost all the tech-
niques adopted for thermo plastics. Ultrason can be
successfully used for applications in which other plas-
tics, e. g. polyamide, polycarbonate, polyoxymethylene
and polyalkylene terephthalates, fail to meet the require-
ments. By virtue of their extraordinary versatility, Ultrason
resins can substitute thermosets, metals and ceramics.
Injection molding of Ultrason
InJECTIOn MOld 05
InJECTIOn-MOldIng PARAMETERS 07
TyPICAl InJECTIOn MOldIng PROBlEMS 09
MAChInE START-UP, InTERRUPTIOn And ShUT-dOwn
PURgIng And ClEAnIng
SAFETy PRECAUTIOnS dURIng PROCESSIng
Injection molding of Ultrason
INjectIoN moLdINg of ULtraSoN
The same basic rules apply to the injection molding of the high performance plastics Ultrason S ( PSU ), Ultrason P ( PPSU ) and Ultrason E ( PESU ) as to other engineering thermoplastics. The most important difference is the signi-ficantly higher processing temperature. Ultrason requires melt temperatures of 330 to 390 C and mold surface tem-peratures of up to 190 C. In addition to suitable machinery and molds these high temperatures also demand careful handling. Some advantages, but also some challenges and possible problems are:
low shrinkage, no after-shrinkage no flashing no untypical corrosion or wear resistance problems Part quality is mostly more important than cycle time good thermal stability no significant influence of residence time on mechanical properties
higher melt temperature higher mold temperature high injection pressure due to high melt viscosity high demolding forces due to good adhesion with metal
Risk of stress cracking due to amorphous character ( holding pressure profile, sufficient mold temperature! )
Silver streaks due to humidity, gate system, feeding air ( high shear )
The presence of even tiny amounts of residual moisture dur-ing processing can adversely affect the quality of Ultrason parts, for example causing silver streaks on the molding surface and foaming of the melt. Problems also arise during plastification of the material.
The predrying of Ultrason should be carried out for three to four hours at 130 to 150 C in dry-air or vacuum dryers to give maximum moisture contents of 0.02 to 0.05 %. Circulat-ing air dryers are unsuitable. For best results moisture levels of below 0.02 % are preferable. Because of the excellent hydrolysis resistance the material drying is only necessary to achieve a perfect surface quality. higher humidity typi-cally has no influence on mechanical properties like impact behavior.
Ultrason granules can absorb moisture very quickly. For this reason the dried material should be fed directly to the injection molding machine.
Ultrason can be processed using three-zone screws which are commonly used with other engineering thermoplastics. Effective screw lengths of 18 to 22 d and pitches of 0.8 to 1.0 d have proven successful. It is advisable to use shallow-flighted screws.
Open nozzles are preferred over shut-off nozzles since their design allows better flow. If shut-off nozzles are used, the best design in terms of flow should be used. In contrast to other thermoplastics it has proven successful when pro-cessing Ultrason to increase the play between the shut-off needle and the guide hole to form a 0.05 to 0.06 mm gap. despite of thermal expansion this should guarantee a suffi-cient clearance even at high temperatures.
5INjectIoN moLdINg of ULtraSoNInjection mold
Because of the high melt viscosity of amorphous thermo-plastics there is no need for very narrow tolerances in parts of the machinery and the mold.
Particular attention should also be paid to the choice of materials for screws, screw tips, barrels, nozzles, and screw couplings. If there is any uncertainty regarding the thermal stability of machine parts, the machine manufacturer should be consulted. generally modern machines are already de-signed for processing temperatures of up to approximately 400 C. In order to allow the processing temperatures of hT (high-temperature) thermoplastics to be achieved reliably heating bands of sufficient heating power are necessary. Barrel temperatures of up to about 400 C cannot always be achieved by means of standard heating bands. Therefore, it is recommended that ceramic heating bands with a specific heating power of about 5 to 8 w/cm2 are used. Otherwise long heating time would lead to higher risk of material deg-radation during every machine start-up.
like the plastification unit the injection mold must also be suitable for relatively high temperatures. Besides the purely mechanical design and choice of suitable materials the main considerations here are optimum design of the cooling channels and their seals and connections by means of heat- and pressure-resistant hoses.
design and material selection
The relatively high operating temperatures must be taken into ac count in the mechanical design of molds. hT thermo-plastics can always be processed using the steels custom-ary for the construction of molds for other engineering ther-moplastics. high-alloyed hot-worked steels ( Table 1 ), which are also suitable for extended use at temperatures of about 200 C, and melt temperatures of above 400 C, have proven successful. Fits and guides must be matched to the in-creased operating temperatures. This is particularly true for combinations of materials of different coefficients of thermal expansion. The metal treatment temperature has to be 50 Kelvin above the afterwards maximum use temperature.
Table 1: high-alloyed hot-worked steels for mold and /or plastifica-tion unit
Steels for unreinforced grades
Steels for reinforced grades with protection against wear
1.2378 1.2379 1.3344
Steels additional corrosion resistance
1.2083 X42Cr13 13 % Cr
like other engineering thermoplastics the production of high-quality moldings in reproducible quality requires opti-mum temperature control of the injection molds. Suitable temperature-control media for achieving mold temperatures from 140 C to about 190 C are both water and oil. The use of water as temperature-control medium is possible to about 200 C with appropriately designed temperature-control equipment. Electrical temperature control may also be possible under certain circumstances.
Bezel for head lamp
molding geometry and gate design
The molding design rules are basically the same as those applicable to other thermoplastics. In the case of Ultrason moldings particular attention should be paid to adequate drafts, transition radii ( 0.4 mm ), and large-area ejector systems. The draft should be at least 1 to 2 for smooth sur-faces. For structured surfaces approximately an additional 1.5 should be provided per 0.02 mm of structure depth. For grades that are optimized for demolding smaller drafts can be possible.
The design rules applicable to other thermoplastics also apply to the design and dimensions of the gating systems. The draft of sprues (half cone angle) should be at least 1.0 to 1.5 . In order to make demolding of the sprue easier the sprue bushing should be well polished. It should be ensured that the transition radius between the sprue and molding is sufficient ( R = 1.0 to 2.0 mm ).
Fog lamp reflector
In pin gates the gate diameter is generally between about 1.5 and 3.0 mm. In tunnel gates the gate diameter should be as small as possible but not less than 0.8 mm. Smaller gates of about 0.4 to 0.8 mm may be possible for small parts and microparts. however, the lowest permissible gate diameter must be checked in each individual case. when designing tunnel gating systems the limited tough-ness in the just-injected state must be noted.
Ultrason can also be processed using hot runner systems. Particular attention should be paid to adequate insulation between the hot runner and the remaining mold. Especially for small gate diameters freezing of the nozzle can occur. Furthermore, dead spots and large pressure losses, caused by excessively narrow runner cross sections, must be avoided under all circumstances.
INjectIoN moLdINg of ULtraSoN
The material temperatures shown in Table 2 have proven successful for the processing of Ultrason. Especially for the combination of high melt temperature and long resi-dence time a rising temperature profile from the feed zone to the nozzle is recommended. The barrel temperature in the first barrel heating zone ( feed zone ) should be between 320 and 360 C. For shorter residence times of the melt in the barrel a horizontal temperature profile may also be appropriate. The hopper region should be maintained at about 60 to 90 C. Figure 1 shows i